Reason for use:
During use, the clutch diaphragm spring will wear on its tip ends at the point where it comes into constant contact with the thrust bearing.
The clutch diaphragm spring in itself is not particularly an expensive item, however, the labour involved in removing the old spring from its housing then replacing it with new will push up the total cost of clutch refurbishment.
By using the Metallisation flamespray process, it is possible to apply a coating of molybdenum onto the work area of the diaphragm spring without removing it from the housing. This makes the spring reserviceable at a fraction of the replacement cost.
Metal spraying molybdenum, using the Metallisation flamespray equipment, gives the unique ability to produce a range of coatings between 250 and 800 HV. This makes it possible to hard face diaphragm springs, giving them added lubrication and valuable extended life.
a) Springs worn below final regrind tolerance should NOT be sprayed. Sprayed metal deposits do not impart any strength to the base material.
b) Components should be checked dimensionally and for cracks or any other major faults.
a) Degreasing. Any approved industrial solvent may be used to completely remove grease or oil from the surface.
b) Preliminary Machining. Grinding or finishing may be used to remove any major scoring on spring tips blending in to form a uniform concentric base.
c) Mask surfaces adjacent to area requiring treatment with a heavy duty masking tape.
d) Thoroughly inspect for contamination prior to blasting.
e) Thoroughly blast with clean Nº 30-36 Grade Aluminium Oxide Grit.
Application of Sprayed Coating
ii. Apply sprayshield masking fluid using a small brush to all areas adjacent to the area to be sprayed. Ensure fluid is not applied to the area being sprayed (small amounts of masking fluid on the area to be sprayed can be removed with an emery cloth).
iii. Thoroughly check the area to be sprayed to ensure it is free from contamination.
iv. Important: The area to be sprayed should not come into contact with oil, grease, hands or any other form of contamination.
NOTE: Masking is not always required when spraying diaphragm springs.
Continue to spray the main deposit of molybdenum (99E), using the same spraying parameters as the bond coat, but increase spray range to 100mm-150mm (4″-6″).
Complete the spraying of the main deposit traversing the spray head to give a uniform coating over spring tips.
The final deposit thickness will depend upon the condition of the spring prior to spraying and should be adjusted accordingly.
Spraying Parameters Metallisation Mark 61
Acetylene Pressure – 1.03 bar / 15 psi
Oxygen Pressure – 1.9 bar / 30 psi
Air Pressure – 4.5 bar / 65 psi
Flowmeter Pointer Settings – Gas 5.5 / Oxygen 2.25
Under normal circumstances it is possible to use the component in the ‘as sprayed’ condition without any problems, but for cosmetic purposes, a light polish may be required.